2Outline Asphalt Binders Asphalt Emulsions Cutback Asphalts Polymer Modified Binders and Performance Based AsphaltAsphalt RubberAggregatesStorage and HandlingSampling Guidelines and Delivery
3Asphalt Binders Paving Asphalt Constituent A complex hydrocarbon mixture consisting primarily of the residue from crude oil refningAsphalt properties depend on its chemical composition, crude source and typeHighly temperature dependentCaltrans requirements for asphalt binders – Section 92 of the Standard Specifications
5Asphalt Binders – Specifications Caltrans used AR (Aged Residue) system for many yearsCaltrans adopted the Performance Graded (PG) system for asphalt binder since 2006 for conventional binders and 2007 for modified binders
6Asphalt Binders – Specifications In the PG system, asphalt is specified by:Dynamic Shear Rheometer (DSR) for performance at high and intermediate temperaturesBending Beam Rheometer (BBR) for performance at cold temperaturesAging CharacteristicsPurity and Safety
7Asphalt Binders – Specifications EquipmentPurposePerformance ParameterRolling Thin Film Oven, RTFOSimulate binder aging during HMA production & constructionResistance to aging during and immediately after constructionPressure Aging Vessel, PAVSimulate binder aging during HMA lifeResistance to aging over the length of pavement service lifeRotational Viscometer, RVMeasure binder properties at high construction temperatureHandling & pumpingDynamic Shear Rheometer, DSRMeasure binder properties (stiffness and elasticity) at high and intermediate service temperaturesResistance to permanent deformation (rutting) and fatigue crackingBending Beam Rheometer, BBRMeasure binder properties at low service temperaturesResistance to thermal cracking
8Complete table available at Asphalt Binders – Specifications - UnmodifiedPerformance Graded Asphalt BinderSpecificationGradePropertyAASHTO Test MethodPG58-22 a64-1064-1664-2870-10Original BinderFlash Point, Minimum °CT48230Solubility, Minimum % bT4499Viscosity at 135°C, cMaximum, Pa·sT3163.0Dynamic Shear,Test Temp. at 10 rad/s, °CMinimum G*/sin(delta), kPaT315581.006470RTFO Test e,Mass Loss, Maximum, %T240RTFO Test Aged BinderComplete table available at
12Asphalt Emulsions Emulsion Constituent Breaking Curing An asphalt dispersed in waterBreakingThe process of separating the asphalt and waterCuringThe process by which the asphalt expels water and dries to a film on the aggregate or surface
14Asphalt Emulsions Emulsion Manufacture Asphalt is sheared into small droplets and coated/reacted with a chemical stabilizer or emulsifierEmulsion must be stored at right pressure and temperature to prevent from damaging
15Asphalt EmulsionsA device used to shear the asphalt – Colloid Mill Cross
17Asphalt Emulsions Emulsifiers Anionic emulsifiers are based on fatty acidsCationic emulsifiers are based on various types of amines. Cationic emulsifiers are used for slow set, rapid, quick sets and micro surfacing of various types of amines depending on the application.Caltrans uses both. The choice between anionic and cationic is based on the application requirements and the characteristics of the aggregate to be used in the mix
18Asphalt Emulsions Caltrans Specifications Anionic emulsions: rapid set (RS), Medium Set (MS), and Slow Set (SS)Cationic emulsions: rapid set (CRS), Medium Set (CMS), and Slow Set (CSS)SubcategoriesPolymer modified emulsionsQuickset slurry emulsion
19Emulsion - Classification TypeSlowSettingMediumRapidAnionicSS-1SS-1hMS-1MS-2MS-2hHFMS-1HFMS-2HFMS-2hHFMS-2sRS-1RS-2HFRS-2CationicCSS-1CSS-1hCMS-2CMS-2hCRS-1CRS-2This table identifies the different emulsion classifications normally used for fog seals, sand seals, and brush seals. The types of emulsions associated with the different surface seals are identified later (under the heading of “Construction”).Q: What is the difference between a “2” and a “1”?A: A “2” signifies a higher residual asphalt than a “1.”Note: If this has been presented in previous modules, use this table as a review.
20Emulsion Classification Names cationicrapid-settingCRS - 2high viscosity(65% asphalt)cationicslow-settingCSS - 1hhard asphalt57% asphaltThis slide explains the different name designations (as explained by ASTM).high-floatHFMS - 2swith solventmedium-setting (anionic)65% asphalt
21Cutback AsphaltsA solution of asphalt in a hydrocarbon solvent (e.g., kerosene, diesel, or naphtha)Solvents are used to reduce the asphalt’s viscosity so that the cutback can be pumped and sprayed at lower temperatures (104 to 293F [40 to 145ºC]) than that required for conventional asphalt
22Cutback AsphaltsIn California, only slow and medium cure cutbacks are still made and only slow cure cutbacks are generally specifiedThe main use for cutbacks is prime coats over aggregate base materials prior to placement of an asphalt-wearing course in new construction
23Cutback Asphalts Manufacture Specifications and Testing Easy Manufactured on site by circulation in a tankIn refinerySpecifications and TestingStandard specifications Section 93 “Liquid Asphalts”Flash point and water content, viscosity, and boiling range of the solvent
24Polymer Modified Binder Polymerslarge molecules that are used to enhance the performances of asphalt cement and asphalt concrete pavement, particularly at high temperatures. Specifications and TestingPolymer Modified BindersStyrene Butadiene Copolymer (radial and linear) (SBS)Polyethylene (PE)Styrene Butadiene Rubber (SBR)Polybutadiene (PB)Ethylene Vinyl Acetate (EVA)Ehtylene Methyl Acrylate (EMA)Atactic Polypropylene (PP)Epoxies and UrethanesTire Rubber (Crumb)
25Polymer Modified Binder Manufacture ProceduresMetering of polymer, asphalt, and additives.Wetting of the polymer by the asphalt/additive blend.Dispersion of the polymer.Allowance for any interaction (reaction) of the polymer with the asphalt.Storage and transportationMost important steps are dispersion and reaction
26Complete table available at Polymer Modified BinderComplete table available at
27Asphalt Rubber Asphalt Rubber Constituent Asphalt rubber manufacture Crumb Rubber Modifier (CRM)Scrap Tire RubberHigh Natural Rubber Content Scrap RubberAsphalt CementExtender oil - CaltransAsphalt rubber manufactureHeat asphalt cement to ~ 375 to 440°FAdd CRM into a pre-wet tankAsphalt contacts and wets CRM particlesAsphalt reacts with rubber particles to form a gel coated particle
28Crumb Rubber Modifier (CRM) SCRAP TIRE1/16” +/- in SizeHIGH NATURAL RUBBER1/32” +/- in Size
31AR PG Asphalt CementsFor high mountain and high desert areas, use PG as the base asphalt.For other areas (coastal, inland valleys, low and south mountain, and low desert) use PG as base asphalt.
32AR Binder Specification ARB: 20 2% CRM content by total binder mass. The CRM must include 25 2% by mass of high natural rubber CRM and 75 2% scrap tire CRM.The scrap tire CRM consists primarily of No. 10 to No. 30 sized particles (2 mm to 600 m sieve sizes). The high natural rubber CRM is somewhat finer, mostly No. 16 to No. 50 (1.18 mm to 300 m sieve sizes).
33AR Binder Specification The extender oil dosage for chip seals ranges from 2.5 to 6% by mass of the asphalt cement. However, the minimum extender oil content for use in RAC mixes may be reduced to one percent to minimize potential for flushing and bleeding for hot climate, high traffic index (TI) locations.
34Aggregates The major building material for pavements Form the structural matrix in AC mixTypesIgneousSedimentary rocksGravelSandsSlag
35Aggregate Properties Chemical Physical Affinity to asphalt Grading or particle size distributionCleanliness or presence of deleterious materialsHardness or abrasion resistanceDurability or soundnessParticle shape and surface textureAbsorption characteristics
37Storage and Handling Conventional asphalt Modified asphalts, including asphalt rubber and MB)Asphalt emulsionsAggregate
38Storage and Handling Conventional asphalt Avoiding Problems during StorageMinimizing the risk of overheatingMinimizing oxidation and loss of volatilesMaintaining asphalt homogeneityMinimizing heat lossStorage and Handling Temperatures and Times are product specific
39Storage and Handling Asphalt Emulsion Handling Storage Pumping – use of appropriate pump to avoid changing the properties of emulsionTemperature – affects the behavior of asphalt dropletsTransport – avoid air enters the emulsion since air can break the emulsionDo not mix cationic and anionic emulsionsStorageThe key is to prevent asphalt particles from settling
43Storage and Handling Tankage Guidelines Bulk tanks should be circulated at regular intervals. Circulation should be done slowly.The frequency of circulation will depend on the weather and how long the emulsion has spent in storage.Most emulsions only require circulation once a week in summer and once every five days during the winter.Circulation should be performed in the middle of the day, not first thing in the morning due to the colder temperatures.
44Storage and Handling Tankage Guidelines The time of circulation is based on the size of the tank; a 1320 gal (5000 L) tank should be circulated for 15 minutes while a 2640 gal (10,000 L) tank requires 20 minutes.Pumps must be flushed after use, but never into the emulsion tank.Lines and pumps should be able to be warmed before use.Lines should not be left part full of emulsion.
45Storage and Handling Cleaning Procedures Flush equipment including hoses thoroughly with WATER.Flush equipment and hoses with kerosene, NOT diesel, distillate or other solvent. These materials may dissolve asphalt but they are also incompatible with the emulsion and may cause the emulsion to break rather than flush it away. NEVER FLUSH INTO THE EMULSION TANK.
46Storage and Handling Cleaning Procedures (cont.) Finish with a second flush with water.If a pump or line is already clogged with bitumen gentle heat may be applied at the blockage. Do not apply heat to the lines, as this will break the emulsion.Soak pumps with kerosene for an hour or more.Flush again with water after blockage is removed.
47Acceptable Switch Load Combination Last Product in TankProduct to be LoadedAsphalt CementCutback AsphaltCationic EmulsionAnionic EmulsionOK to LoadEmpty to No Measurable QuantityCrude Petroleum and Residual Fuel OilsAny Product Not Listed AboveTank Must be Cleaned
48Aggregate Storage and Handling Stockpile areas should be clean and stable to avoid contamination from the surrounding area.Stockpiles should be on free draining grades to avoid moisture entrapment.Stockpiles should be separated for different aggregate sizes to prevent inter-mingling.
49Aggregate Storage and Handling Segregation may be avoided by avoiding stockpiling in a cone shape. Acceptable stockpile shapes are either horizontal or radial. Making each end dump load a separate pile, each adjacent to the next, makes horizontal stockpiles. Radial stockpiles are made with a radial stacker.Degradation of the aggregate creating fines can be avoided by handling the stockpile as little as possible. In chip seal or slurry surfacing applications, re-screening may be considered.
50Sampling GuidelinesSamples of emulsion and binder shall be taken in conformance with the requirements in AASHTO T 40, “Sampling Bituminous Materials,” and Section 8-01 and 8-02 of the Construction Manual and California Test Method 125Observe safety proceduresSample binders daily using new, clean, dry 0.26 gal (1 L) cans with screw lidsSamples are normally taken from the application lance at the rear of the distributor. Drain off sufficient material through the nozzle to ensure removal of any material lodged there
51Sampling GuidelinesSamples should be taken after one-third and not more than two-thirds of the load has been removedDo not submerge sample containers in solvent or wipe containers with solvent saturated cloths. Use a clean, dry cloth, only immediately after sampling, to clean containersAttach a Sample Identification Form (TL-0101) to each material sample in accordance with Section 8-01 of the Construction Manual and instructions printed on the TL-0101 bookletProvide the address of the Resident Engineer on the TL-0101
52Sampling GuidelinesEmulsions have a shelf life; therefore, it is important that all samples be sent to the Transportation Laboratory dailyAggregates should be sampled according to the contractual requirementsSamples of aggregate shall be taken according to Section “Proportioning” of the Standard SpecificationsSamples may be taken from a conveyor belt or sampling chute.Field samples must be taken from the stockpile. AASHTO T 2 and Section of the Standard Specifications (9) describe the method
53Sample DeliverySamples for testing are to be delivered to the Transportation Laboratory:Materials Engineering and Testing ServicesFlexible Pavement Materials Branch, MS #55900 Folsom BoulevardSacramento, California
54Summary Asphalt Binders Asphalt Emulsions Cutback Asphalts Polymer Modified Binders and Performance Based AsphaltAsphalt RubberAggregatesStorage and HandlingSampling Guidelines and Delivery